A COMPARATIVE EVALUATION OF
FLUORIDE RELEASE AND SHEAR BOND STRENGTH OF A
POLYACID - MODIFIED COMPOSITE RESIN,
A RESIN MODIFIED GLASS IONOMER CEMENT AND A
CONVENTIONAL COMPOSITE RESIN
An Invitro Study
Dissertation submitted to
THE TAMILNADU DR. M.G.R. MEDICAL UNIVERSITY
in partial fulfillment of the degree of
MASTER OF DENTAL SURGERY
BRANCH - V ORTHODONTICS
C E R T I F I C A T E
This is to certify that Dr. SANGEETHA DURAISAMY, post graduate student
(2002-2005) in the Department of Orthodontics, Tamil Nadu Govt. Dental College & Hospital,
Chennai-03 has done this dissertation titled “A COMPARATIVE EVALUATION OF
FLUORIDE RELEASE AND SHEAR BOND STRENGTH OF A POLYACID - MODIFIED COMPOSITE RESIN, A RESIN MODIFIED GLASS IONOMER CEMENT AND A CONVENTIONAL COMPOSITE RESIN - An Invitro Study” under our direct guidance and supervision in partial fulfillment of the regulations laid down by the Tamilnadu Dr. M.G.R.
Medical University, Chennai, for M.D.S., (Branch – V Orthodontics) Part - II degree
Dr. L. MUTHUSAMY, M.D.S.,Professor & Head
Dept. of Orthodontics
Tamil Nadu Govt. Dental College & Hospital,
Chennai – 600 003.
Dr. W.S. MANJULA, M.D.S., Additional Professor
Dept. of Orthodontics
Tamil Nadu Govt. Dental College & Hospital, Chennai – 600 003.
Dr. T.R. SUDARSAN, M.D.S.,
I wish to express my sincere & heartfelt gratitude to Dr.L.Muthusamy, M.D.S, Professor and Head of the Department, Department of Orthodontics, Tamil Nadu Government Dental College and Hospital, Chennai – 3 for his constructive criticism, ceaseless support and continuous encouragement throughout my post graduate studies.
I consider it my privilege & honour, to acknowledge with deep sense of gratitude, my sincere thanks to Dr.W.S.Manjula,M.D.S., Additional Professor, Department of Orthodontics, Tamil Nadu Government Dental College and Hospital, Chennai – 3, for her immense help and valuable guidance in making this work possible.
I am grateful to Dr.T.R.Sudarsan M.D.S., Principal, Tamil Nadu Government Dental College and Hospital, Chennai – 3 for having permitted me to conduct the study.
My sincere thanks to Dr.C.Karunanidhi,M.D.S., Additional Professor, Department of Orthodontics for his encouragement.
I wish to express my gratefulness to Dr.G.Vimala,M.D.S., Dr.S.Premkumar,M.D.S., and
Dr.J.Nagalakshmi,M.D.S., Assistant Professors, Department of Orthodontics, for their valuable suggestions and encouragement.
I am extremely thankful to Mr. Kulasekaran, Chief Water Analyst, Mrs. Chandrika, Tamilnadu Water Supply and Drainge Board, Chennai for helping me in estimating fluoride release.
Dr.J.Kaladharan, M.V.Sc., Ph.D., Assistant Professor, Department of Animal Genetics, Madras Veterinary College for his guidance in stereomicroscopic evaluation.
I thank Mr.Mathai, for helping me in statistical part of my study.
I would like to convey my special thanks and appreciation to Mr. Hussain and Mr.Sameer,
Citi Dot Net for their meticulous contributions in typing the dissertation.
I would like to acknowledge the never ending support and help rendered by my friends, juniors and colleagues.
My heartfelt thanks to my beloved mother, my husband and my family for standing by me whenever I needed them most.
Sl.No. Title Page No.
1. Introduction 1
2. Aims and Objectives 6
3. Materials and Methods 7
4. Review of Literature 20
5. Results 61
6. Discussion 64
7. Summary and Conclusion 71
L I S T O F T A B L E S
1. Mean Fluoride release of all the six groups
2. Tukey HSD analysis of group A,C,E at day 1, 7, and 30
3. Tukey HSD analysis of group B,D,F at day 1, 7, and 30
4. Student’s independent t-test between group A & B, C&D and E&F at day 1.
5. Student’s independent t-test between group A & B, C&D and E&F at day 7
6. Student’s independent t-test between group A & B, C&D and E&F at day 30.
7. Student’s paired t-test of group A & B between day 1, 7 and 30.
8. Student’s paired t-test of group C & D between day 1, 7 and 30.
9. Student’s paired t-test of group E & F between day 1, 7 and 30.
10. Descriptive statistics for shear bond strength values.
11. ANOVA of Group I, III, and V.
12 Tukey HSD of Group I, III, and V.
13. ANOVA of Group II, IV and VI.
14. Tukey HSD of Group II, IV and VI
15. Student’s independent t-test between group I & II, group III & IV and group V & VI.
L I S T O F T A B L E S
17. Shear stress (Mpa) required for various probability of failure
18. Analysis of ARI score results of Chi-square test
19. Spearmen rank correlation analysis between bond strength and ARI scores
LIST OF GRAPHS
1. Mean shear bond strength of six sample groups
2. Weibull curve for Python
3. Weibull curve for Transbond XT
4. Weibull curve for Fuji Ortho - LC
L I S T O F P H O T O G R A P H S
1. Adhesive materials
2. Adhesive sample disks stored in distilled water and artificial saliva
4. TISAB III solution
5. Fluoride ion specific combination electrode
6. Python light cure adhesive
7. Transbond XT
8. Fuji ortho – LC
10. Light cure unit
11. Brackets bonded to teeth samples mounted on acrylic blocks
13. Instron universal testing machine
14. Tooth sample mounted on instron universal testing machine
15. Stereo microscope
For the past 50 years, since the introduction of acid etching by Buonocore21
in 1955 major improvements were achieved in bonding brackets to the teeth. The pioneering work of Buonocore, Bowen 17,18, Wilson130 and Tavas121 were
instrumental in developing procedures and materials that have led to present day standards in orthodontic adhesives.
Buonocore advocated the use of phosphoric acid etching to improve the adhesion of acrylic resin filling materials to enamel as early as 1955.59 This
procedure involves dissolution of the organic component of the enamel matrix, creating microporosities in the enamel surface. Etching increases the wettability of the surface and facilitates the penetration of the resin into the enamel. A mechanical bond is formed between the resin adhesive and the tooth. In 1964 Newman87 first bonded Orthodontic brackets to the teeth using the acid etch
technique and an epoxy derived resin.
Bisphenol A glycidyl dimethacrylate, a diacrylate resin more commonly known as Bowen’s resin or bis GMA, was patented in 196218. This resin is an
Decalcification of enamel surface adjacent to orthodontic brackets is a common adverse effect of orthodontic treatment53,56. Increased plaque
accumulation with concomitant bacterial acid production results in decalcification of the surrounding enamel. Patients often have difficulty in maintaining adequate oral hygiene with orthodontic appliances attached directly to the teeth. Estimates of the presence of white spot lesions per patient in orthodontically treated
population range from 12.6 percent to 50 percent.56
This persistent problem has stimulated a search for a preventive procedure. Programs for prevention of decalcification or caries in the dental field are usually directed toward one or more of the following factors (1) alteration of the oral flora, (2) decrease in frequency and quality of fermentable carbohydrate intake, and (3) increase in resistance of the tooth surface to demineralization.25
Recently, studies have been concerned with the latter factor, by attempting to decrease the surface solubility. The benefits of fluoride in prevention of tooth decay and remineralization of decalcified enamel were described in the dental literature as early as 1942. The mechanism of fluoride reducing decalcification or caries is multifactorial. Fluoride increases the resistance of enamel to acid,
increases the maturation rate of enamel, and interferes with the metabolism of microorganisms. Recent evidence shows that fluoride may facilitate the
calcium fluoride and fluorapatite crystals. This reaction enhances remineralization of the etched enamel making it more resistant to demineralization5, 90.
Patient compliance with self-administered fluoride delivery system is generally poor126. Attempts have been made to develop bonding agents that release
fluoride. Such adhesives include glass ionomer cements, resin modified glass ionomer cements (RMGIC), and poly acid modified composite resins (PAMC)126.
The potential advantage of a bracket bonding material with sustained release of fluoride is that a continuous release of fluoride would be possible adjacent to the bracket, the area of greatest risk for decalcification31 .
Wilson and Kent introduced glass polyalkenoate, glass ionomer cements, to dentistry in 1972130. Glass ionomer cements bonds by carboxyl chelation to
and dentin. GIC hydrogel phases are thought to be responsible for the uptake and re-release of added environmental fluoride from topical gels, rinses, and dentifrices 86. Low fracture resistance limits their orthodontic use primarily to band
Tavas and Watts first described the use of visible light to cure composites used in orthodontic bonding in 1979121. In response to the demand for
improvement in bond strength of the conventional glass ionomer cement, Antonucci et al introduced resin modified glass ionomer cements (RMGICs) in 19887.Addition of 10% to 20% resin monomers to the glass ionomer cements
resulted in a cement that is initially hardened with the use of either light or chemical activators to polymerize the monomers. Resin modified glass ionomer cements are adhesive cements with improved physical properties and more stable hydrogels compared with glass ionomer cements. Polymerization of the resin monomers hastens the initial hardening of resin modified glass ionomer cements without interfering significantly with the acid-base setting reaction, the fluoride release, or the chelation of carboxyl groups to metal and tooth surfaces86.
occurs because water is absent from the composition. However, after light-activation of the compomer, it is postulated that water sorbs into the compomer, allowing a delayed acid-base reaction that may release fluoride and other
remineralizing ions from the aluminosilicate glass. The relatively weak acid-base reaction does not result in increased physical properties of the compomer. The absence of hydrogels restricts ion uptake and release, although fluoride recharging of compomers has been reported and can be explained by water sorption and diffusion dynamics2,32,101,133. Compomers have been linked to caries inhibition in
vitro because of fluoride release from the aluminosilicate glass filler at low pH. Carboxyl chelation with cations on enamel, dentin, and metallic surfaces has not been shown to occur with compomer adhesives. Acid etching or other surface treatment and dry enamel surface are pre requisites for bonding with poly acid modified composite resins. Physical properties are acquired quickly as
compomers polymerize, and their early setting strengths are superior to those of the resin modified glass ionomers but inferior to those of the resin adhesives2.
A recently introduced bonding material Python light cure adhesive (TP orthodontics, LaPorte, Indiana) a polyacid modified composite resin126 is marketed
with manufacturer’s claim of fluoride release and improved bond strength.
AIMS AND OBJECTIVES
1. To evaluate the amount of fluoride release from a polyacid modified composite material (Python light cure adhesive,TP orthodontics, LaPorte, Indiana) stored in distilled water and artificial saliva using a Fluoride ion specific combination electrode and to compare it with a fluoride releasing control, resin modified glass ionomer cement (Fuji Ortho LC, GC, Tokyo, Japan ) and a non fluoridated composite resin control (Transbond XT, 3M Unitek, Monrovia, Calif).
2. To evaluate the shear bond strength of the Python Light cure adhesive (TP orthodontics, LaPorte, Indiana) using the Instron universal testing machine
and to compare it with the controls resin modified glass ionomer cement (Fuji Ortho LC, GC, Tokyo, Japan) and a non fluoridated composite resin control (Transbond XT,3M Unitek, Monrovia, Calif).
3. To evaluate the site of bond failure and the amount of adhesive remaining on the debonded tooth surface (Adhesive remnant index) using
MATERIALS AND METHODS
I. ESTIMATION OF FLUORIDE RELEASE
All the three materials used in this study were light-cured orthodontic
bracket-bonding adhesives, two of them releasing fluoride
Python light cure adhesive (TP Orthodontics, Inc., LaPorte, Ind).
This is a light-cured polyacid modified composite resin system releasing fluoride that is recommended for use to bond brackets on an uncontaminated etched enamel surface.
Transbond XT (3M Unitek, Monrovia, Calif).
This is a light-cured composite resin system that is recommended for use to bond brackets on an uncontaminated etched enamel surface.
Fuji Ortho LC (GC, Tokyo, Japan).
This is a light cured resin modified glass ionomer cement releasing fluoride recommended for use to bond brackets on an unetched enamel surface.
Preparation of adhesive disc samples
Twenty discs (6 mm in diameter and 2 mm in thickness) were
fabricated from each material Python light cure adhesive, Transbond
XT, and Fuji Ortho LC, using a split mold following manufacturer’s
be 0.9425 cm2
. After light curing, each polymerized specimen was
released from the mold and placed into a polyethylene test tube. Half
of the test tubes (10 per type of material) received 1 ml of distilled
water, and the other half received 1 ml of artificial saliva. All test
tubes were then capped, labeled, grouped and stored in an incubator at
37°C and 100% relative humidity.
Group A - Python light cure adhesive disc samples stored in 1ml of
Group B - Python light cure adhesive disc samples stored in 1ml of
Group C - Transbond XT light cure adhesive disc samples stored in 1ml of
Group D - Transbond XT light cure adhesive disc samples stored in 1ml of
Group E Fuji Ortho LC light cure adhesive disc samples stored in 1ml of
Group F Fuji Ortho LC light cure adhesive disc samples stored in 1ml of
The artificial saliva was made up according to a research based
and contained 1.04 g/L of KCl, 0.68 g/L of NaH
0.42 g/L of NaHCO3
0.03 g/L of CaCl2,
and 0.01 g/L of MgCl
.The pH of the artificial saliva was 6.95.
Fluoride ion-specific combination electrode
Measurements of fluoride released were taken with a fluoride
ion-specific combination electrode (model EA 940; Orion Research Inc,
Beverly, Mass). The electrode was calibrated with a series of standard
fluoride solutions, ranging in concentration from 0.1 to 1000 ppm
Total Ionic Strength Adjustment Buffer
Total Ionic Strength Adjustment Buffer TISAB III (Orion Research
Inc.) is a commercial buffering solution designed to keep the pH
between 5 and 5.5; it also frees F - bound to hydrogen ions,
eliminating interference from other ionic species such as hydroxyl and
Three ml of TISAB III (Orion Research Inc) was added to each ml of
sample solution diluted to 30 ml, to obtain a constant background ionic
strength and eliminate aluminium interference. Readings in mg/ lr were
directly noted from the ion meter.
Fluoride in 1ml of the sample (mg/lr) =
The values in ppm were then converted to µg/cm 2 by dividing by the
surface area of the discs.
1 ppm = 1mg / lr = 1µg /ml
Measurements of the fluoride levels and changing of the solutions
were carried out daily for the first 7 days, end of every week for 3
weeks, and again at the end of first month using the
ion-specific combination electrode.
One day before each weekly and monthly fluoride assays, the
specimens were washed and transferred into 1 ml of fresh solution, to
avoid cumulative effects, and 24 hours later fluoride release data were
gathered for the different time intervals.
Descriptive statistics, including the mean, standard deviation, were calculated for each of the six groups of the samples tested. ANOVA, Tuckey – HSD and Student’s t test were used to determine the statistical significance of difference between mean fluoride release of each group with categorical variations being the type of material, type of storage media and time of estimation.
Hundred and twenty human premolars extracted for orthodontic treatment purpose were collected, cleaned of debris and stored in distilled water. The water was changed weekly to avoid bacterial growth. The criteria for tooth selection included, intact buccal enamel, with no hypoplastic spots, caries or cracks due to the pressure of the extraction forceps, and not subjected to any pretreatment chemical agents, such as alcohol, formalin, hydrogen peroxide.
Three different types of adhesive systems were evaluated in the current study, Python light cure adhesive (TP Orthodontics, Inc., LaPorte, Ind), a light-cured polyacid modified composite resin system releasing fluoride that is recommended for use to bond brackets on an uncontaminated etched enamel surface.
Transbond (3M Unitek, Monrovia, Calif), a light-cured composite resin system that is recommended for use to bond brackets on an uncontaminated etched enamel surface.
Fuji Ortho LC (GC, Tokyo, Japan).
Hundred and twenty, Gemini Series (3M Unitek, Monrovia, Calif.), Roth prescription 0.022” slot, premolar metal brackets with an average bracket base surface area of 10.61 mm2 were used in this study.
Instron universal testing instrument
Instron universal testing instrument, (Model 1195, Instron Corp., Canton, Mass.) which was calibrated to a full-scale compression load range of 0.1KN to 100KN was used in this study to determine the shear bond strength. The Instron machine has a lower vise to which the testing samples can be secured and a upper crosshead which can move either upwards or downwards with variable speed, to which a chisel with sharp edge can be connected to produce the shearing force for debonding the brackets in shear bond strength testing. The force applied to debond the bracket was recorded with a pen on the x-y recorder connected to the Instron machine, with force recorded on the y-axis and time on the x-axis. The highest point on the graph is the bond strength of the adhesive in kilograms.
The hundred and twenty premolars were separated randomly into six groups of twenty each. All teeth were embedded in self-cure acrylic blocks of cuboid shape up to the level of the cementoenamel junction. . The acrylic blocks were made from standardized molds and fashioned to fit the Instron universal testing machine. Each tooth was oriented such that the buccal surface is
perpendicular with the bottom of the mold, with the long axis of the crown parallel to the central axis of the acrylic block and when oriented with the testing device the buccal surface will be parallel to the force during the shear strength test. The acrylic blocks were colour coded for easy identification of the different groups.
Group I.: (blue colour blocks) Brackets to be bonded using Python light cure adhesive. Bond strengths to be tested 30 minutes after bonding, after completion of initial polymerization.
Group II: (yellow colour blocks) Brackets to be bonded using Python light cure adhesive. Bond strength s to be tested 24 hours after bonding, after completion of final polymerization.
Group III: (light pink colour blocks) Brackets to be bonded using Transbond XT adhesive. Bond strengths to be tested 30 minutes after bonding, after completion of initial polymerization.
adhesive. Bond strength s to be tested 24 hours after bonding, after completion of final polymerization.
Group V: (green colour blocks) Brackets to be bonded using Fuji Ortho LC adhesive. Bond strength to be tested 30 minutes after bonding, after the completion of initial polymerization.
Group VI: (clear acrylic blocks) Brackets to be bonded using Fuji Ortho LC adhesive. Bond strength to be tested 24 hours after bonding after completion of final polymerization.
Groups I and II represented the new polyacid modified composite resin material releasing fluoride. Whereas groups III through VI were control groups, representative of the conventional light-cured resin adhesive systems and a resin modified glass ionomer cement.
The teeth were cleaned and then polished with a non-fluoridated oil free pumice paste and rotating rubber prophylactic cup in a slow-speed hand piece for 10 seconds. The teeth were then rinsed with a water spray and dried with a blast of air from oil-free air source.
Python light cure adhesive was used to bond the brackets to group I and II teeth samples. Bonding procedures were performed according to the
enamel conditioner, a resin sealant and a bonding paste. The enamel conditioner was applied to the buccal surface of each tooth for 35 seconds. The teeth were then rinsed with a water spray for 30 seconds and dried with an oil and moisture free air source for 20 seconds. The buccal surfaces of the treated teeth appeared chalky white in color. A thin coat of the resin sealant was applied to the enamel surface and to the bracket base. The bonding paste was placed and spread on the bracket base with a spatula. The bracket was then firmly placed on the tooth. Any excess paste around the bracket base was removed with an explorer. The brackets were exposed to the light source for 30 seconds with 15 seconds each on mesial and distal side of the bracket, approximately 5mm above the interproximal contact area using a Hilux curing unit (Heraeus kulzer, Germany).
placed and spread on the bracket base with a spatula. The bracket was then firmly placed on the tooth. Any excess paste around the bracket base was removed with an explorer. The brackets were exposed to the light source for 20 seconds with 10 seconds each on mesial and distal side of the bracket, approximately 5mm above the interproximal contact area using a Hilux curing unit (Heraeus kulzer,
Fuji Ortho light cure adhesive was used to bond the brackets to group V and VI teeth samples. Bonding procedures were performed according to the manufacturer’s instructions. Powder and Liquid were dispensed in the standard powder to liquid ratio of 3.0g/1.0ml. The powder was divided into 2 equal parts and the first portion was mixed with the liquid for 10 seconds. Then the remaining powder was mixed thoroughly for an additional 15 seconds. The mix was placed and spread on the bracket base with a spatula. The tooth surface to be bonded was wiped with a moist cotton pellet because a desiccated enamel surface will adversely affect the bond strength. The bracket was then firmly placed on the tooth. Any excess paste around the bracket base was removed with an explorer. The brackets were exposed to the light source for 40 seconds with 10 seconds each on mesial, distal, occlusal and gingival aspect of the bracket, using a Hilux curing unit (Heraeus kulzer, Germany).
37°C until testing. At the end of 30 minutes, group I, III and group V samples were subjected to shear strength analysis on an Instron machine. Group II, IV and group VI samples were subjected to shear strength analysis after 24 hours.
Shear bond strength testing
Each sample was subjected to shear bond strength testing on an Instron universal testing machine. The acrylic block was secured in the lower vise of the Instron with the surface of the bracket base parallel to the line of force. A chisel was connected to the upper crosshead of the Instron such that its sharp edge can be placed between the bracket base and enamel and a shearing load can be applied on the enamel bracket interface when the upper crosshead moves downwards.
An occlusogingival load was applied to the bracket producing a shear force with a 50KN load cell and a crosshead speed of 1 mm/minute until shearing of the bracket from the tooth occurred. The shearing force required was recorded on the x-y recorder with force recorded on the y-axis with a scale of 20 kg and time on the x-axis. The highest point on the graph is the bond strength recorded in kilograms. The values are converted to newtons and then to megapascals using the surface area of the bracket base and recorded.
1 kg = 9.81 newtons 1Mpa = 1newton / mm2
Adhesive Remnant Index
After debonding, the teeth were rinsed and dried using an air water syringe. No attempt was made to remove any remaining adhesive until the teeth were subjected to Adhesive Remnant Index assessment. All the 120 samples were examined with a stereomicroscope under 20X magnification to evaluate the site of bond failure and the presence of residual adhesive. Any adhesive remaining after removal of the bracket was assessed according to the Adhesive Remnant Index (ARI) as given by Artun and Bergland, and scored on a scale of 0 = No adhesive left on the tooth, 1 = Less than half of the adhesive remaining on the tooth surface, 2 = More than half of the adhesive remaining on the tooth surface, 3 = All of the adhesive remaining on the tooth surface, showing the impression of the bracket base.
REVIEW OF LITERATURE
New orthodontic adhesive resins and hybrid composite resins offer
improved physical properties like greater bond strength and clinical benefits like release of fluoride and prevention of enamel decalcification due to plaque
accumulation around orthodontic appliances. This review of literature was made as an attempt to highlight the physical properties, chemical characters and clinical performance of composite resin bonding adhesives, Glass ionomer bonding
adhesives, resin modified glass ionomers and polyacid modified composite resin with emphasis on their fluoride releasing property and shear bond strength.
Buonocore M.G (1955)21’59 introduced the bonding technique in the field of
dentistry. He demonstrated that pretreatment of enamel surface with orthophosphoric acid increased the surface area of enamel and produced
mechanical inter locking of resin to enamel. He employed a phosphoric acid and phosphomolybdate oxalic acid treatment to alter enamel surface chemically and concluded that phosphoric acid treatment gave better results.
Bowen R.L. (1962)17,18 explored the possibility of using epoxy resins
(diglycidyl ether of bisphenol A) mixed with silica particles. The in vitro results were promising, but the presence of moisture inhibited the polymerization process of the epoxy resin. To overcome this problem, Bowen attached methyl
epoxy resin to a dimethacrylate. The experimental outcome was successful and resulted in new resin called Bisphenol A glycidyl methacrylate, or BIS-GMA, or Bowen’s resin.
Newman G.V. (1965)87 introduced the direct bonding technique by
combining acid etching with epoxy resin for bonding orthodontic brackets.
Balenseifen JW, Madonia JV. (1970)13 stated that fixed orthodontic appliances
retains plaque ,makes oral hygiene maintenance difficult and are responsible for
further demineralization reactions.
Gwinnett AJ, Buonocore MG, Sheykholeslam Z. (1972)58 suggested that
topical fluoride applications fill in the interprismatic spaces produced by acid etching and may act as a physical barrier and thus reduce the bonding capacity of the adhesives.
Sheykholeslam and associates (1972)111 reported that topical application
of sodium fluoride (NaF), stannous fluoride (SnF2), titanium tetrafluoride (TiF4),
and zirconium tetrafluoride (ZrF4) after acid etching decreased the tensile bond
strength of a methyl methacrylate resin.
Miura et al (1973)84 measured shear bond strengths of plastic brackets
surface which has been hypothesized to inhibit optimum etching from occurring.
Kochavi D, Gedalia I, Anaise J. (1975)71 evaluated the effect of
conditioning with fluoride and phosphoric acid on enamel surfaces by scanning
electron microscopy and concluded that topical fluoride treatments could cause
significant reductions in bond strength.
Reynolds (1975)106 suggested that minimum bond strength of 6-8 Mpa
would appear to be adequate for most clinical orthodontic needs. He also reported successful clinical bonding with adhesives that provide invitro bond strength of approximately 5 Mpa.
Jeansonne BG, Feagin FF. (1979)66 showed that fluoride was more
effective in inhibiting demineralization of the enamel than increasing
remineralization of lesions, supporting the in vitro observation that low levels of
fluoride in acidic buffer solutions decrease the solubility of the enamel
Ceen, and Gwinnett, (1980)23 conducted a study to determine the thickness
Hirce JD et al (1980)60 have found that application of basic phosphate
fluoride or 8% stannous fluoride did not alter the bond strength of the resin adhesive.
Gorelick, Geiger, and Gwinnett(1982)56 studied the incidence and
severity of white spots after a full term of orthodontic treatment among patients in the separate private practices of two of the authors. Results showed that 50 percent of the patients experienced an increase in white spots. 10 per cent of the teeth had white spots in the treatment group compared to 2.5 per cent in the control group. Certain teeth and tooth surfaces exhibit a predisposition to white spot formation. Access to the flow of saliva and the distance from bracket to free gingival margin are factors affecting formation of white spot lesions. They also concluded that teeth banded or bonded for a relatively short treatment interval (from 12 to 16 months) showed the same incidence of white spots as those involved in longer treatment (as long as 36 months).
Mellberg JR, Mallon DE. (1984)82 following an in vitro study stated that
sodium mono fluoro phosphate and sodium fluoride accelerated remineralization of small decalcified or carious lesions and also reduced the formation of new lesions by incorporation of fluoride into the enamel structure as fluorapatite [Ca5(PO4)3F]
conventional resin after conditioning the enamel surface with 37% phosphoric acid and crystal growth conditioning with polyacrylic acid and found that polyacrylic acid has less bond strength. They used an Adhesive Remnant Index (ARI) system to evaluate the amount of adhesive left on the tooth after debracketing. This index system was developed on the basis of a pilot study on twenty extracted teeth, and the criteria are as follows: a score of
0 = No adhesive left on the tooth,
1 = Less than half of the adhesive remaining on the tooth surface, 2 = More than half of the adhesive remaining on the tooth surface,
3 = the entire adhesive remaining on the tooth surface, showing the impression of
the bracket base.
Read M.J.F (1984)105 described about the bonding of orthodontic
attachments using a visible light cured, urethane dimethacrylate resin. He mentioned that the light cured resin has generous working time and on command set, which makes removal of excess material easy. The homogenous consistency of the composite remains constant over a long period of time and this makes handling more predictable.
Barkmeier, Gwinnett, and Shaffer, (1985)14 conducted an in vitro study
differences were observed in surface morphology of the etched site.
Evans and Powers (1985)42 studied the bond strength of no mix
orthodontic cements and recommended the minimal and uniform thickness of resin cement for maximal strength for bonding. They stated that bond strength decreases as thickness increases, because of a greater amount of thermal expansion, polymerization shrinkage, trapped volatiles, and imperfections (voids and cracks) When one-step or no-mix cements were used, the depth of cure at the primer-paste interface was also found to be an important factor as thickness was increased.
Norris et al (1986)89 evaluated the retentive bond strengths of orthodontic
bands cemented with two new fluoride-releasing cements, a zinc polycarboxylate
and a glass ionomer, and compared them with the retentive bond strength of bands
cemented with the standard orthodontic cement zinc phosphate. They also
evaluated the site of cement failure. They concluded that under the test conditions,
both the zinc polycarboxylate and glass ionomer cements tested are as effective as
the standard orthodontic luting cement, zinc phosphate, in retaining bands. They
stated that the favourable failure site of the glass ionomer cement may offer
clinical protection against decalcification under loose orthodontic bands. The
adequate working time of the glass ionomer cement is equivalent to that of the
zinc phosphate; however, the short working time of the zinc polycarboxylate
White (1986)128 described a method of bonding orthodontic brackets to the
enamel surfaces of teeth with glass ionomer cement. He emphasized the necessity for drying the teeth with cotton rolls and isolating the newly bonded brackets from mouth moisture during the early stage of glass ionomer setting. White also stated that the glass ionomers used in his evaluation were not as strong as composite resins. The article stressed the need to avoid early saliva contamination and to use only very light arch wires immediately after the bonding procedure, because the material did not achieve full strength for at least 24 hours.
Reilly and Featherstone (1987)90 conducted a study to investigate the
amount and extent of demineralization occurring around bonded orthodontic appliances after one month in vivo and the ability of commercially available fluoride products to inhibit and/or reverse such orthodontically related demineralization. He concluded that rapid demineralization occurs around the orthodontic appliances as early as one month, even with the use of a proven fluoride dentifrice. He also stressed the importance of use of additional preventive measure against orthodontically related decay.
Geiger AM et al (1988).53 In a clinical study to evaluate the effect of
Øgaard, Rølla, Arends,Ten Cate (1988)96 performed clinical experiments
to investigate the effect of fluoride on carious lesion development and on lesions
established during fixed orthodontic therapy. They stated that all presently
available fluoride agents are developed from the concept of fluoridating the
enamel in the form of fluorhydroxyapatite but research has indicated, that calcium
fluoride formation may be a major aspect of the mechanism of the cariostatic
effect of topical fluoride. Therefore they compared a fluoride solution with very
low pH (1.9) that induced large amounts of calcium fluoride with a 0.2% solution
of sodium fluoride (NaF). They found that daily fluoride mouth rinsing with a
0.2% solution of sodium fluoride (NaF) retarded lesion development significantly,
whereas the fluoride solution with low pH inhibited lesion formation completely.
Øgaard, Rølla, Arends (1988)94 conducted experiment to investigate
carious lesion development associated with fixed orthodontic therapy. Visible
white spot lesions were seen within 4 weeks in the absence of any fluoride
supplementation. Both micro radiographic and SEM examinations showed surface
softening of the enamel surface. They concluded that the enamel demineralization
associated with fixed orthodontic therapy is an extremely rapid process caused by
a high and continuous cariogenic challenge in the plaque developed around
brackets and underneath ill-fitting bands and recommended careful inspection of
the appliance at every visit and preventive fluoride programs are therefore
Greenlaw R, Way DC, Khadry AG. (1989)57 stated that although the in
vitro shear bond strength of visible light cure is only one half that of the
chemically cured resin, the visible light-cured resin can be used clinically with good results and the enamel loss with visible light cure was also less during debonding procedure.
Artun and Thylstrup (1989)11 conducted a three year clinical and SEM
study of surface changes of carious enamel lesions after debonding of orthodontic
appliances. They confirmed that surface wear rather than repair causes the clinical
improvement in arrested white spot lesions and fluorides alone cannot prevent
caries development if the status of the cariogenic challenge is preserved. It is
therefore equally important to concentrate on hygiene measures combined with
regular professional plaque removal.
Klockowski, Davis, et al (1989)70 evaluated the bond strength and
Ogaard B. (1989)95 studied the prevalence of white spot lesions in
19-year-olds subjected to and not subjected to orthodontic treatment. Fifty-one orthodontic
patients at an average of 5.7 years since orthodontic appliances were removed and
47 untreated subjects were examined. The median white spot score was
significantly higher in the orthodontic group than in the untreated group. The
orthodontically treated subjects also had more teeth with white spot lesions than
the untreated subjects. The highest prevalence was noted on the first molars in
both groups. In the orthodontic group the mandibular canines and premolars and
the maxillary lateral incisors were also affected. The present study showed that
white spot lesions after orthodontic treatment with fixed appliances may present
an esthetic problem, even more than 5 years after treatment
Sonis. A. and Snell (1989)5 conducted a study to compare a visible
light-activated, fluoride-releasing bonding system with a visible light-activated conventional bonding system relative to bracket retention and prevalence of decalcification in twenty-two patients with 206 experimental brackets and 206 control brackets over an average treatment period of 25 months and concluded that a visible light-activated, fluoride-releasing bonding system is capable of adequately retaining brackets while aiding in the prevention of decalcification around bonded appliances
O’Brien, Read et al., (1989)91 evaluated the clinical performance of visible
that visible light-cured adhesive was a satisfactory alternative to conventional chemical cured materials. The handling properties of the light-cured materials were found to be superior to the chemically cured materials.
Underwood and colleagues (1989)123stated that incorporation of inorganic
fluorides into dental resins creates problems of phase separation and loss of
mechanical integrity because of the highly polar nature of the fluoride salts and
low polarity of dental resins. Organic fluoride incorporation has a plasticizing
effect that also yields poor properties. He conducted a study to examine the
clinical durability and caries inhibition potential of a fluoride-exchanging resin
when used as an orthodontic bracket-bonding adhesive and to compare it with a
non fluoride releasing adhesive. This fluoride-releasing resin is unique in that the
fluoride ion is incorporated as a mobile ion charge in an anion-exchanging resin.
This resin has a three-dimensional, highly crossed-linked network with fixed
positive charges and fluoride counter charges. Fluoride release occurs when
fluoride ions are exchanged for other anions in the oral environment. Rather than
supplying fluoride to the oral environment by material dissolution, the fluoride is
given up in exchange for other anions and the structure integrity of the resin is
maintained. Long-term low-level fluoride release is possible without reduction in
necessary physical characteristics. They demonstrated a 93% reduction of
occurrence of dark zone (2% to 4% enamel porosity) formation around brackets
first stages of enamel alteration. They concluded that the sustained low-level
release of fluoride ions from the fluoride-exchanging adhesive reduced the
formation and progression of very early demineralization of enamel surrounding
orthodontic appliances and occurrence of adhesive rather than cohesive failure
indicated that structural integrity was maintained for both adhesives. Success and
failure rates of both adhesives indicated similar durability characteristics.
Cook P.A. (1990) 28Compared the vivo bond strength of glass ionomer
cement with a composite resin-bonding agent. The results of his evaluation indicated that the bond strength of the glass ionomer was not nearly as good as that of the composite resin. Cook stated that thorough drying of the teeth before glass ionomer use was not necessary but that cotton rolls should be used to isolate the field of operation. He also concluded that glass ionomer bonded relatively better to the bracket than to the enamel; its fractures tended to be cohesive failures, within the cement itself.
El Mallakh BF, Sarkar NK. (1990)40 evaluated the fluoride release from
glass-ionomer cements in de-ionized water and artificial saliva and concluded that
the fluoride release from material into distilled water is significantly greater than
that into artificial saliva
Fajen et al. (1990)43 evaluated the bond strength of three glass ionomer
glass ionomers to be significantly less.
Fox NA. (1990)47Stated that the low-dose fluoride continually released
exactly where it is needed may, however, be more important in the prevention of
decalcification through fluorapatite formation than single high doses of fluoride
Joseph and Rossouw (1990)124 stated that fully polymerized, fissure
sealants could be used to seal the complete buccal enamel, thus preventing the
possibility of immediate or future decalcification around orthodontic brackets.
They also determined the shear bond strengths of stainless steel orthodontic
brackets bonded to teeth with an orthodontic bonding resin together with a primary
coating of various fissure sealants (a light-cured unfilled clear fissure sealant, a
light-cured microfilled fissure sealant, and a chemically cured opaque fissure
sealant.) and evaluated the fracture sites of these debonded samples. This study
demonstrated that a fissure sealant resin can be applied to seal the buccal surface
of a tooth and have a bracket bonded to it, which exhibits shear bond strengths that
are equal to, if not higher than, the standard method of bonding, and the fracture
sites of the fissure-sealed teeth are located more at the resin/enamel interface than
those of teeth without sealant, thus leaving less cleaning of the tooth surface after
Fox NA, McCabe JF, (1991)46 compared the shear bond strength of a
glass ionomer cement. The results obtained showed that the conventional
composite resin had the highest mean bond strength. The results were analyzed
using the weibull analysis, which examines bond reliability rather than mean bond
strength. They concluded that the bond reliability of the conventional composite
resin and fluoride releasing composite resin are comparable and both of them will
behave in a similar manner in the clinical situation.
McCourt et al (1991) 76conducted a study to evaluate the bond strength of
two light cured fluoride-releasing materials, a urethane dimethacrylate with
sodium fluoride (time Line) and a glass ionomer-linked methyl methacrylate
(Vitra bond) when used as an orthodontic bracket adhesive and compared them
with a non-fluoride-releasing light-cured composite resin bonding material
(Transbond). They concluded that the two fluoride-releasing, light-cured materials
tested have low bond strengths after 30 days and are not acceptable as orthodontic
bracket bonding agents. They recommended a modified bracket bond method in
which a thin layer of fluoride-releasing low-viscosity material is placed around the
brackets already bonded in patients with a high caries risk or poor oral hygiene
Rezk-Lega et al. (1991)107 conducted an in vitro study of glass ionomers
have significantly less bond strength than composite resin in vitro.
Bjorn Ogaard, felipe Rezk – Lega et al (1992)93 designed a study to
investigate the cariostatic potential in vivo of an visible light curing adhesive for the bonding, of orthodontic brackets and found that the fluoride adhesive reduced lesion depths by 48% than the non fluoride adhesive and it was concluded that the regular use of tooth paste was insufficient to inhibit lesion development around orthodontic brackets.
Compton et al. (1992)26 compared the bond strength of glass ionomer
cements, emphatically stating that they must not be contaminated by moisture during the bonding procedures. In addition, they suggested, conditioning the tooth bond sites with a weak acid to enhance the cohesive strength.
Eliades et al (1992)41 explained two basic concepts adopted in the design of
fluoride-releasing composite resins: the incorporation of fluoride in a dispersed
phase, which is released by dissolution and the synthesis of fluoride-releasing
resins in which fluoride is given by an ion-exchange mechanism and stated that
these approaches demonstrated the problems associated with the rate of fluoride
release and with the solubility of the polymer network. He evaluated the extent of
fluoride uptake from enamel bonded to an experimental visible light-cured
orthodontic adhesive based on a new fluoride releasing system, based on ytterbium
dispersive electron probe microanalysis to study the enamel-adhesive interfaces
and concluded that the cumulative fluoride uptake by enamel from the
experimental adhesive was not statistically different from the fluoride detected in
the control groups
Fricker (1992)50 conducted a twelve month clinical trial of a glass ionomer
cement for the direct bonding of orthodontic brackets compared with a standard
composite bonding adhesive. This study shows a significant difference in failure
rates of orthodontic brackets cemented with a thick mix of glass ionomer (20%)
compared with composite bonding resin (5%). He concluded that glass ionomer
cement, when used as a thick mix, has a poor clinical performance than composite
resin for the direct bonding of orthodontic brackets. The leach of fluoride by glass
ionomer cement prevents enamel demineralization around bracket margins and is a
definite advantage and these cements should be reserved as bracket adhesives for
patients who have poor oral hygiene and high caries rate.
Tanbirojn D et al (1992)120 reported that with a F release of as little as 0.2
µgF-/cm2, a F uptake in the outer 10 µm of enamel, after 24 hours contact, of as
high as 5400 ppm occurs.
McKnight-Hannes C, Whitford GM. (1992)78 in a study estimating the
the fluoride release from three glass-ionomer materials and the effect of varnishing
affected by several factors such as temperature, mechanical shaking, frequency of
analysis as well as the medium in which the samples are stored.
Aasrum E, Nganga PM, Dahm S, Ogaard B. (1993)1 compared the
tensile bond strength of a fluoride releasing light cure adhesive with two light cure
adhesives and concluded that the fluoride-releasing light-curing adhesives for
bonding brackets gave tensile bond strength adequate for orthodontic purposes.
The bond strength did not change during a 6-month period when fluoride was
released from the material and such a fluoride-releasing adhesive may be of
clinical interest to inhibit white spot lesions around brackets.
Axel Voss, Reinhard Hickel, Stefan Mölkner (1993)12 conducted a study
to measure in vivo the bonding properties of conventional mesh-backed brackets
bonded with GIC, and he also evaluated a new experimental bracket base
designed to improve bond strength with GIC. The results of this study showed that
GIC is suitable for use as a bonding material for orthodontic attachments
providing bond strength that can be improved by developing modified bases.
Boyd RL (1993)19 while comparing three self-applied topical fluoride
preparations for control of decalcification in orthodontic patients found that significant decalcification occur in patients, even when they had received
Dubroc, Mayo, and Rankine (1994)38 examined the ability of a
fluoride-releasing resin to reduce caries, as well as demineralization around orthodontic brackets, by using the Sprague-Dawley rat as a model. The results of this study suggest that in the rat model a fluoride-releasing orthodontic adhesive has the capacity to reduce the extent of decalcification in the immediate vicinity of plaque retentive orthodontic brackets and reduce incidence of caries at sites distant from the point of application, by serving as a source for controlled release of fluoride throughout the oral cavity.
Fox NA, McCabe JF, (1994)48 reviewed a large number of publications on
point of application and direction of debonding force is the same for all specimens. At least 20 and preferably 30 specimens must be used per test. Site of failure should be reported. Statistical analysis should include survival analysis to give a prediction of the performance of the material, which can be related to the clinical situation. Bond strengths should be quoted either in Newtons or Megapascals. They concluded that equally valid arguments can be made for alternative methods of bond strength testing and the above suggestions has been made as they are relatively easy to carry out, minimize the specimen preparation and have been used widely and by confirming to one technique valid comparisons of attachments and materials can be easily made offering more guidance to the clinical orthodontist.
Fricker, (1994)51 worked with glass ionomer cement and found the same
rate of success in bonding brackets to enamel surfaces as he did with composite cements, When a dentine conditioner was applied on tooth for ten seconds, then rinsed, followed by lightly drying the tooth surfaces before bonding the brackets with the glass ionomer cement.
Silverman, Cohen et al (1995)113 explained the use of a new light-cured,
activator. The resin component was actually a mixture of three monomers with 2-hydroxyethyl-methacrylate (HEMA) being the major constituent, and a camphorquinone photoinitiator. The HEMA provides for a sharp setting reaction of the material when exposed to visible light irradiation.
Sinha PK, Nanda RS, Ghosh J. (1995)114 presented a indirect bonding
technique with a thermal-cured, fluoride-releasing resin. He stated that this resin
combined advantages of adequate clinical bond strength, placement accuracy, and
ease of clean-up after bonding and debonding with the ability to release fluoride.
Wiltshire and Janse van Rensburg(1995)129 evaluated fluoride release
from two nonfluoride visible light-cured orthodontic adhesives, as well as two fluoride-containing visible light-cured orthodontic adhesives. They polymerized ten circular disks, with a volume of 56.57 mm3 and a surface area of 0.94 cm2 of
from fluoride release from orthodontic adhesives reduced the decalcification during fixed orthodontic treatment.They explained that the release of fluoride from the nonfluoride adhesives could possibly be due to small amounts of
fluorides such as barium fluoride, present in the inorganic phase of the adhesives.
Larry J. Oesterle.(1995)92 conducted a study to determine whether
increasing the curing time or the setting time increases the shear bond strength of a visible-light-cured orthodontic adhesive (Trans Bond XT). The results indicated that the shear bond strength was nearly 5kg on average for the samples exposed to 20 seconds of curing and allowed to set for two minutes. Extending the setting time to five minutes produced more than a 20% increase in bond strength. However, waiting 20 or 30 minutes resulted in only small additional increments of strength (7% and 8%, respectively). Strength after 24 hours is more than double that after two minutes and nearly 50% greater than after 30 minutes. They also concluded that increasing the curing time increases the shear bond strength.
Rashid Ahmed Chamda, Errol Stein (1996)102 evaluated the bond
strength achieved with a light-cured bonding system at selected time intervals over
a 24-hour period and compared with the bond strengths produced by a chemically
cured system over a similar period. The bond strengths for the chemically cured
system were initially low, but these increased with time because of the continued
polymerization of the resin under the bracket base. The light-cured sample
application of orthodontic forces, and these bond strengths also increased with
time. . This increase was due either to a dual cure system in the formulation of the
resin or to the polymerization of the resin under the bracket base after the diffusion
of free radicals. The in vitro shear/peel bond strengths obtained with a light-cured
resin at 2 minutes and 5 minutes after curing were significantly greater than those
produced by a chemically cured resin at the similar time periods. There was no
significant difference between the bond strengths achieved by the chemically
cured and light-cured systems at the 10-minute, 60-minute, and 24-hour intervals.
E. Nkenke et al (1997),88 conducted an experimental study to determine
the tensile bond strength of stainless steel, ceramic and plastic brackets bonded to the bovine enamel using a conventional two-paste orthodontic bonding resin(Concise), a light-cured, fluoride-releasing adhesive (Sequence), a no-mix-orthodontic bonding resin(system I) and a light-curing glass ionomer cement (Photac Fil). For evaluation of the experimental data the Weibull analysis was applied.
Pramod K. Sinha, Ram.S. Nanda et al (1997)100 stated that sustained
fluoride-releasing composite resins have the potential to prevent decalcification of
enamel that may occur during the course of orthodontic treatment. They evaluated
the potential of two matrix-bound fluoride-releasing adhesives (MBF) for
orthodontic use by comparing the shear bond strengths and remnant adhesive on
orthodontic adhesives. They concluded that fluoride releasing light and self-cured
orthodontic bonding adhesives have favourable bond strengths and ARI scores
when compared with nonfluoride-releasing versions and fluoride-releasing
orthodontic adhesives may prove to be clinically useful orthodontic bonding
Agneta Marcusson et al (1997)3 conducted study to test the benefit from
using glass ionomer cement (AquaCem) instead of a conventional diacrylate (Unite) in bracket bonding for the prevention of white spot formation. They concluded that the use of a GIC for orthodontic bonding would result in a significant reduction in the number of white spot surfaces at debonding compared with the use of conventional diacrylate. Although markedly reduced in both groups, the number of affected surfaces was still higher 2 years after debonding than before treatment.
Ortendahl, B. Thilander, and M. Svanberg (1997)119 investigated the
levels of streptococcus mutans in plaque adjacent to orthodontic brackets retained with glass ionomer and a resin based composite after full term orthodontic treatment and found that the mean levels of these microorganisms were lower in plaque adjacent to glass ionomer retained brackets compared to composite retained brackets.
system that used a hybrid adhesive containing a resin reinforced glass ionomer (Fuji Ortho LC,) and compared it with a more traditional light-cured bonding system (Transbond,) that contained resin material only. The shear bond strength was performed after thermal cycling between 5° ± 2° C and 50° ± 2° C for a total of 2000 cycles. They concluded that with etched enamel, even when contaminated with water or saliva before bonding, the newly introduced light-cured resin-reinforced glass ionomer adhesive system has comparable shear bond strength, as the traditional light-cured composite resin systems. . With unetched enamel, the shear bond strength of the resin-reinforced glass ionomer adhesive is significantly reduced by a third to a half. This reduction in bond strength is critical and should be taken into consideration by the clinician, because the residual bond strength might not be able to withstand the forces produced during routine clinical orthodontic procedures.
Stephen J. Lippitz et al(1998)116 evaluated and compared the shear bond
were statistically lower in magnitude compared with the composite resin bonding adhesive when the enamel surfaces were not etched with polyacrylic acid.
Hugo R. Armas Galindo, Lionel Sadowsky,et al(1998)62 conducted an
invivo longitudinal clinical study to evaluate and compare the rate of success and/
or failure between a visible light-cured bonding material and a chemically cured
bonding material using both systems in every patient by bonding contralateral
quadrants with each system respectively. Results showed that the failure rate of
the visible light-cured composite was 11.3% and that of the chemically cured
composite was 12% with no statistically significant differences between the failure
rates of the two systems.
Susan AI-Khateeb, Carl-Magnus Forsberg et al (1998)117 stated that
be blocked with mineral and result in a more pronounced diffusion inhibition.
Geurstsen W, Leyhausen G, Garcia – Godoy F. (1999)55 measured the
surface microhardness (Vickers) as well as the release of fluoride from four polyacid modified composite resins (Compoglass F, F 2000, Dyract AP, experimental compomer) after storage in various artificial saliva (buffers) including one esterase buffer. Concluded that the action of salivary esterase may weaken the surface of poly acid- modified composite resin restorations. As a clinical consequence, wear may be enhanced and load resistance may be reduced. In addition, fluoride release from polyacid modified composite resins may be increased by hydrolytic enzymes in saliva and under acidic conditions.
Itota T, Okamoto M, et al (1999)63 investigated the release and recharge
non-fluoride releasing resin composite gave any evidence of recharge. Resin modified glass ionomers, and polyacid modified composite resins affected by acid buffer solution could not recharge much fluoride even if they were immersed in the1000 ppm F NaF solution. The results suggested that the matrix of resin modified glass ionomers and polyacid modified composite resins functioned as a reservoir of fluoride, but the functions were lost as a result of acid attack.
Meehan .P.M et al (1999)81 conducted a study to determine the in vitro
shear bond strength (in megapascals) and location of bond failure with two light-cured glass ionomer resin systems (Fuji Ortho LC ) and ( Ultra Band Lok ) and to compare them with a light-cured composite resin control (Transbond XT). They concluded that even though new generation of resin-modified GICs showed improved bond strength over conventional glass ionomer cement adhesives, they do not appear to provide sufficient shear bond strength. They suggested that the addition of a mechanical bond through enamel conditioning to the chemical bond might provide clinically acceptable bond strength.
Stephanie.E. Steckel, Frederick. A. Ruggerberg, Gray M. whitford (1999)115 compared the three types of adhesives on enamel (No mix, chemically
Bishara. E.S., Leigh Von Wald et al (2000)16 conducted a study to
determine the effects of increasing the light cure time on the initial shear bond strength (in the first half an hour) of a resin modified glass ionomer adhesive (Fuji Ortho LC). Results showed that the resin reinforced glass ionomer adhesive has a significantly lower bond strength in the first half an hour after bonding when compared to a conventional resin adhesive(Trans Bond XT) and the initial strength of the glass ionomer adhesive was significantly, increased by increasing the light cure time for an additional 5-10 seconds. The mean increase in shear bond strength between 5 and 10 seconds of additional light curing was not significant but the variability was less with the longer cure time.
Jeremy Knox et al (2000)67 conducted a study to determine the resilience,
ionomer cement offered a reduced energy absorbing capacity immediately after bracket placement and reduced cohesive and mechanical adhesive strength.
Millett D.T. et al (2000)32 studied the invivo survival time and cariostatic
zotential of a compomer (Dyrect Orthodontic) and compared it with a composite resin bonding material (Right on). They concluded that the survival time distributions of brackets bonded with compomer or resin adhesive appear comparable but bonding with compomer reduced decalcification of enamel significantly.
Owens S.E. et al (2000)98 evaluated the shear bond strength and site of
Yip. HK, Smales RJ. et al (2000)133Conducted a study to compare the
fluoride ion release from a freshly mixed polyacid modified resin composite, or compomer (Dyract) and three resin modified glass ionomer cements (Fuji II LC, Photac-Fil, and Vitremer) and to compare the use of 3 units for measuring fluoride release.Fluoride measurements were carried out using a fluoride ion-selective electrode connected to a pH ion-selective electrode meter. Fluoride ion release was measured in parts per million, micrograms per square centimeter, and micrograms per cubic millimeter. Showed Fuji II LC, Photac-Fil, and Vitremer showed high initial release values which decreased exponentially and then showed a slow decline during the ensuing time. Dyract released significantly less fluoride ions during the first 84 days than did the three resin – modified glass ionomer cements and maintained this low level of release throughout the study period. The amounts of fluoride ion release measured at any time interval varied with the units of measurements chosen but the pattern of release remained the same. They concluded that there was a wide variation in the amounts of fluoride ions released from related products, but the patterns of release were similar and unaffected by the units of measurements used.
Alexander S.A. and Ripa L.W (2000)4 conducted a study to compare the
effectiveness of tooth brushing followed by fluoride rinsing, fluoride gel brushing,
or fluoride gel dentifrice brushing alone in controlling the demineralization that